Statistical optimization of guest uptake in crystalline sponges: grading structural outcomes.
Carroll, Robert C.; Coles, Simon J.; IUCrJ 11 (2024) –; doi:10.1107/S2052252524004871

data_1571883
_publ_section_title
;
 Statistical optimization of guest uptake in crystalline sponges: grading
 structural outcomes.
;
_journal_coeditor_code           LT5068
_journal_issue                   4
_journal_name_full               IUCrJ
_journal_paper_doi               10.1107/S2052252524004871
_journal_volume                  11
_journal_year                    2024
_chemical_formula_moiety         'C36 H24 I6 N12 Zn3'
_chemical_formula_sum            'C36 H24 I6 N12 Zn3'
_chemical_formula_weight         1582.18
_chemical_name_systematic        phenyl(p-tolyl)methanone
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2024-03-26
_audit_creation_method
;
Olex2 1.5-alpha
(compiled 2024.02.16 svn.r378c4104 for OlexSys, GUI svn.r6928)
;
_cell_angle_alpha                90
_cell_angle_beta                 102.4170(10)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   35.2498(4)
_cell_length_b                   14.90120(10)
_cell_length_c                   31.3590(4)
_cell_measurement_reflns_used    16768
_cell_measurement_temperature    100.00(10)
_cell_measurement_theta_max      69.1830
_cell_measurement_theta_min      2.6110
_cell_volume                     16086.5(3)
_computing_cell_refinement       'CrysAlisPro 1.171.42.72a (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.72a (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.72a (Rigaku OD, 2022)'
_computing_molecular_graphics    'Olex2 1.5-alpha (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5-alpha (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2016/6 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      100.00(10)
_diffrn_detector                 'hybrid pixel array detector'
_diffrn_detector_area_resol_mean 10
_diffrn_detector_dtime           0.000
_diffrn_detector_type            'Rigaku, HyPix Arc-100'
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
--------------------------------------------------------------------------
  1  \w    112.00 146.00   0.50    4.00    --   83.39  74.00 -67.00   68
  2  \w     21.00  97.00   0.50    4.00    --   83.39 -74.00 163.00  152
  3  \w    109.00 155.00   0.50    4.00    --   83.39  37.00 -90.00   92
  4  \w     37.00  98.00   0.50    4.00    --   83.39 -77.00-120.00  122
  5  \w     12.00  42.00   0.50    4.00    --   83.39 -37.00 150.00   60
  6  \w     92.00 142.00   0.50    4.00    --   83.39   0.00 -90.00  100
  7  \w     40.00  66.00   0.50    4.00    --   83.39 -77.00 120.00   52
  8  \w     17.00  42.00   0.50    4.00    --   83.39 -37.00 -90.00   50
  9  \w     12.00  38.00   0.50    4.00    --   83.39 -37.00  60.00   52
 10  \w     38.00  82.00   0.50    4.00    --   83.39   0.00 -90.00   88
 11  \w     80.00 121.00   0.50    4.00    --   83.39  57.00-120.00   82
 12  \w     12.00  37.00   0.50    4.00    --   83.39 -37.00   0.00   50
 13  \w     23.00  48.00   0.50    4.00    --   83.39 -57.00 -90.00   50
 14  \w     14.00  44.00   0.50    4.00    --   83.39 -37.00-180.00   60
 15  \w     74.00 123.00   0.50    4.00    --   83.39  57.00  60.00   98
 16  \w     12.00  42.00   0.50    4.00    --   83.39 -37.00 -30.00   60
 17  \w    -93.00 -34.00   0.50    4.00    --  -79.34  74.00 -67.00  118
 18  \w   -122.00 -67.00   0.50    4.00    --  -79.34 -74.00 163.00  110
 19  \w   -135.00 -90.00   0.50    4.00    --  -79.34 -99.00 -60.00   90
 20  \w    -34.00  -9.00   0.50    4.00    --  -79.34  37.00 150.00   50
 21  \w   -139.00-114.00   0.50    4.00    --  -79.34 -99.00 -90.00   50
 22  \w   -115.00 -89.00   0.50    1.60    --  -55.07 -74.00 163.00   52
 23  \w    -80.00 -41.00   0.50    1.60    --  -55.07 -74.00 163.00   78
 24  \w    -30.00   7.00   0.50    1.60    --  -55.07  74.00 -67.00   74
 25  \w    -23.00   7.00   0.50    1.60    --  -55.07  19.00 -60.00   60
 26  \w    -24.00  14.00   0.50    1.60    --  -55.07  19.00-120.00   76
 27  \w     -5.00  29.00   0.50    1.60    --   52.07 -74.00 163.00   68
 28  \w     52.00  77.00   0.50    1.60    --   52.07  74.00 -67.00   50
 29  \w    -12.00  27.00   0.50    1.60    --   52.07 -19.00-180.00   78
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_details 'Rigaku, UG2 \k goniometer'
_diffrn_measurement_device_type
; Rigaku 007HF diffractometer equipped with Arc)Sec VHF Varimax confocal
 mirrors and a UG2 goniometer and HyPix Arc-100 detector
;
_diffrn_measurement_method       'profile data from \w-scans'
_diffrn_measurement_specimen_support 'MiTeGen loops'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0339811000
_diffrn_orient_matrix_UB_12      0.0567892000
_diffrn_orient_matrix_UB_13      -0.0253746000
_diffrn_orient_matrix_UB_21      0.0033977000
_diffrn_orient_matrix_UB_22      0.0628437000
_diffrn_orient_matrix_UB_23      0.0396555000
_diffrn_orient_matrix_UB_31      0.0289461000
_diffrn_orient_matrix_UB_32      0.0592639000
_diffrn_orient_matrix_UB_33      -0.0176906000
_diffrn_radiation_collimation    0.3
_diffrn_radiation_monochromator  'Arc)Sec VHF Varimax focusing mirrors'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0222
_diffrn_reflns_av_unetI/netI     0.0185
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       42
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       35
_diffrn_reflns_limit_l_min       -37
_diffrn_reflns_number            68924
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         68.249
_diffrn_reflns_theta_min         2.567
_diffrn_source                   'Rotating anode'
_diffrn_source_current           30.0
_diffrn_source_power             1.2
_diffrn_source_target            Cu
_diffrn_source_type              'Rigaku 007 HF'
_diffrn_source_voltage           40.0
_exptl_absorpt_coefficient_mu    19.316
_exptl_absorpt_correction_T_max  0.467
_exptl_absorpt_correction_T_min  0.222
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.72a (Rigaku Oxford Diffraction, 2022)
Analytical numeric absorption correction using a multifaceted crystal
model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.307
_exptl_crystal_description       block
_exptl_crystal_F_000             5856
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.06
_refine_diff_density_max         0.504
_refine_diff_density_min         -0.364
_refine_diff_density_rms         0.054
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.088
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     598
_refine_ls_number_reflns         14633
_refine_ls_number_restraints     21
_refine_ls_restrained_S_all      1.091
_refine_ls_R_factor_all          0.0362
_refine_ls_R_factor_gt           0.0302
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0540P)^2^+5.8687P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0925
_refine_ls_wR_factor_ref         0.0952
_reflns_Friedel_coverage         0.000
_reflns_number_gt                11920
_reflns_number_total             14633
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            lt5068.cif
_cod_data_source_block           4_mbp_50_10_96b
_cod_database_code               1571883
_shelx_shelxl_version_number     2016/6
_chemical_oxdiff_formula         '(Zn3 I6 N12 H24 C36) (C14 H12 O)2 (C6 H12)4'
_chemical_oxdiff_usercomment     4-methylbenzophenone
_shelx_estimated_absorpt_t_max   0.390
_shelx_estimated_absorpt_t_min   0.205
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Restrained distances
 I303-Zn32 \\sim I403-Zn42
 with sigma of 0.02
 I304-Zn32 \\sim I404-Zn42
 with sigma of 0.02
 Zn32-N305 \\sim Zn42-N305
 with sigma of 0.02
 I303-I304 \\sim I403-I404
 with sigma of 0.04
 I303-N305 \\sim I403-N305
 with sigma of 0.04
 I304-N305 \\sim I404-N305
 with sigma of 0.04
 I302-Zn31 \\sim I402-Zn41
 with sigma of 0.02
 I301-Zn31 \\sim I401-Zn41
 with sigma of 0.02
 Zn31-N301 \\sim Zn41-N301
 with sigma of 0.02
 I302-I301 \\sim I402-I401
 with sigma of 0.04
 I302-N301 \\sim I402-N301
 with sigma of 0.04
 I301-N301 \\sim I401-N301
 with sigma of 0.04
 I306-Zn33 \\sim I406-Zn43
 with sigma of 0.02
 I305-Zn33 \\sim I405-Zn43
 with sigma of 0.02
 Zn33-N306 \\sim Zn43-N306
 with sigma of 0.02
 Zn33-N307 \\sim Zn43-N307
 with sigma of 0.02
 I306-I305 \\sim I406-I405
 with sigma of 0.04
 I306-N306 \\sim I406-N306
 with sigma of 0.04
 I306-N307 \\sim I406-N307
 with sigma of 0.04
 I305-N306 \\sim I405-N306
 with sigma of 0.04
 I305-N307 \\sim I405-N307
 with sigma of 0.04
3. Others
 Sof(I403)=Sof(Zn42)=Sof(I404)=1-FVAR(1)
 Sof(I303)=Sof(I304)=Sof(Zn32)=FVAR(1)
 Sof(I402)=Sof(Zn41)=Sof(I401)=1-FVAR(2)
 Sof(I302)=Sof(I301)=Sof(Zn31)=FVAR(2)
 Sof(I405)=Sof(Zn43)=Sof(I406)=1-FVAR(3)
 Sof(I306)=Sof(I305)=Sof(Zn33)=FVAR(3)
4.a Aromatic/amide H refined with riding coordinates:
 C302(H302), C335(H335), C301(H301), C310(H310), C311(H311), C336(H336),
 C317(H317), C314(H314), C318(H318), C313(H313), C315(H315), C312(H312),
 C331(H331), C322(H322), C323(H323), C330(H330), C319(H319), C333(H333),
 C320(H320), C332(H332), C304(H304), C328(H328), C329(H329), C305(H305)
;
_smtbx_masks_void_probe_radius   1.2
_smtbx_masks_void_truncation_radius 1.2
_shelx_res_checksum              12474
_shelx_hkl_checksum              97915
_shelx_fab_checksum              92389
_olex2_date_sample_data_collection 2024-03-19
_olex2_date_sample_submission    2024-03-19
_olex2_submission_original_sample_id '4-Methylbenzophenone 50_10_96b'
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
- B-factor correction
;
_oxdiff_exptl_absorpt_empirical_full_max 3.206
_oxdiff_exptl_absorpt_empirical_full_min 0.502